[en] In an increasingly environmentally conscious society, there is a need to reduce the consumption and environmental impact of the non-renewable high-performance polymers used in today's life due to their versatility and better properties than other materials such as mechanical and thermal. In this context, in this Master's thesis materials composed of the thermoplastic elastomer called styrene-b- (ethylene-co-butylene)-b-styrene (SEBS) and a renowable filler agent called cellulose were developed with the intention of maintaining, and even improving, its most significant properties for potential applications such as the automotive industry and sensors. Cellulose was selected because of its great interest in the industrial field caused by different reasons: it is a natural source and, also, considerably reduces the production cost despite the fact that it generally contributes to the deterioration of certain properties. This results in the search for a balance between all these qualities. In addition, in polymer blends it is important to consider their chemical nature, which must be similar. Because of their characteristics: SEBS is hydrophobic and cellulose hydrophilic, one of the two materials must be modified. Therefore, two types of modifications were studied: cellulose derivatives with apolar groups to be similar to apolar SEBS and the maleic anhydride grafted SEBS (SEBS-g-MA) to increase its polarity. Once the most suitable materials were selected, a series of SEBS and SEBS-g-MA based films were prepared in which the different celluloses were incorporated with different concentrations, and a study of the morphological, structural, mechanical, thermal and electrical properties was carried out using various techniques: Scanning Electron Microscopy (SEM), Fourier Transform Infrared Spectroscopy (FTIR), tensile testing, Differential Scanning Calorimetry (DSC), Thermogravimetryc analysis (TGA) and dielectric measurements. This made it possible to identify which cellulose precursors and charge contents are the most suitable and interesting from the SEBS applicability point of view. In the morphological characterisation, the immiscibility of the materials was observed, as well as the existence of voids between the filler and the matrix, becoming more noticeable with the increasing of the filler agent content. This caused a decrease in the mechanical properties of the blends films compared to the pure copolymer film due to the lower stress transfer, although, depending on the materials, these properties loss is of different degree. Regarding the thermal properties, the immiscibility was reflected by the occurrence of each characteristic temperature with almost no change. Thermal stability also decreased due to the introduction of the biopolymer with lower resistance to degradation. However, the filling agent caused a positive effect on the electrical properties so that the conductivity increased. In the case of SEBS and ethylcellulose blends, since the decrease in elongation at break and Young's modulus compared to the other films was minor, while the electrical properties were improved, these blends were concluded to be the most promising. Finally, with the idea of obtaining a sustainable material with similar properties to commercial EC, the aim was to extract cellulose from agricultural waste such as poplar and functionalise it by adding bromoethane. The extraction and functionalisation was followed using TGA and FTIR techniques in order to confirm that the desired product was obtained. These techniques established that parameters such as the concentration of sodium hydroxide and temperature not only help the method but also degrade the cellulose, so it is necessary to deal with different parameters until the product is obtained with a viable yield.

[es] En una sociedad cada vez más concienciada con el medioambiente, surge la necesidad de reducir el consumo e impacto ambiental de los polímeros no renovables de alto rendimiento tan utilizados en la vida actual debido a su versatilidad y a sus propiedades superiores a otros materiales, entre ellas mecánicas y térmicas. En este contexto, en el presente Trabajo Fin de Máster se desarrollaron materiales compuestos por el elastómero termoplástico estireno-b-(etileno-co-butileno)-b-estireno (SEBS) junto a la celulosa como agente de relleno renovable con la intención de mantener, e incluso mejorar, las propiedades más significativas para potenciales aplicaciones, tales como en la industria automotriz y en sensores. Se seleccionó la celulosa ya que posee un gran interés en el ámbito industrial al ser de origen natural y además disminuye considerablemente el coste de producción a pesar de que contribuye en general al deterioro de ciertas propiedades. Esto tiene como consecuencia la búsqueda de un equilibrio entre todas estas cualidades. Además, en las mezclas de polímeros es importante tener en cuenta su naturaleza química, que debe ser similar. Debido a que el SEBS es hidrofóbico y la celulosa hidrofílica, uno de los dos materiales debe ser modificado. Por lo tanto, se estudiaron dos tipos de modificaciones: derivados de la celulosa con grupos apolares para ser semejantes al SEBS apolar y SEBS funcionalizado con anhídrido maleico (SEBS-g-MA) para incrementar su polaridad. Una vez seleccionados los materiales más adecuados, se prepararon una serie de films a base de SEBS y SEBS-g-MA donde se incorporaron las diferentes celulosas con distintas concentraciones, y se llevó a cabo un estudio de las propiedades morfológicas, estructurales, mecánicas, térmicas y eléctricas, mediante diversas técnicas: Microscopía Electrónica de Barrido (SEM), Espectroscopía Infrarroja por Transformada de Fourier (FTIR), ensayo de tracción, Calorimetría Diferencial de Barrido (DSC), Termogravimetría (TGA) y medidas dieléctricas. Esto permitió identificar qué precursores de celulosa y contenidos en carga son los más adecuados e interesantes desde el punto de vista de la aplicabilidad del SEBS. En la caracterización morfológica se observó la inmiscibilidad de los materiales, así como la existencia de huecos entre el relleno y la matriz, volviéndose más notables con el incremento del contenido del agente de relleno. Esto causó una disminución en las propiedades mecánicas de los filmes de las mezclas en comparación con el filme del copolímero puro debido a la menor transferencia de tensión, aunque en función de los materiales la pérdida de estas propiedades es de diferente grado. En relación a las propiedades térmicas, la inmiscibilidad quedó reflejada con la aparición de cada temperatura característica sin apenas modificación. La estabilidad térmica también disminuyó debido a la introducción del biopolímero con menor resistencia a la degradación. No obstante, el agente de relleno causó un efecto positivo en las propiedades eléctricas de manera que la conductividad se incrementó. En el caso de la mezcla SEBS y etilcelulosa (EC), dado que la disminución de la elongación a rotura y del módulo de Young en comparación con el resto de filmes fue de menor importancia mientras que las propiedades eléctricas fueron mejoradas, se concluyó que estas mezclas eran las más prometedoras. Finalmente, con la idea de conseguir un material sostenible con propiedades similares a la EC comercial, se trató de extraer celulosa a partir de residuos agrícolas como es el chopo y funcionalizarla mediante la adición de bromoetano. La extracción y funcionalización se siguieron mediante las técnicas TGA y FTIR con la función de confirmar la obtención del producto deseado. Mediante estas se estableció que se debe tener en cuenta que parámetros como la concentración de hidróxido de sodio y la temperatura no solo ayudan al método sino también degradan la celulosa, por lo que es necesario tratar con diferentes parámetros hasta la obtención del producto con un rendimiento viable.